General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.85 - 7.86 g/cm³ Show Material materials with Density of 7.85 - 7.86 g/cm³ |

50.0 °C | 7.84 g/cm³ Show Material materials with Density of 7.84 g/cm³ | |

100.0 °C | 7.82 g/cm³ Show Material materials with Density of 7.82 g/cm³ | |

150.0 °C | 7.81 g/cm³ Show Material materials with Density of 7.81 g/cm³ | |

200.0 °C | 7.79 g/cm³ Show Material materials with Density of 7.79 g/cm³ | |

250.0 °C | 7.77 g/cm³ Show Material materials with Density of 7.77 g/cm³ | |

300.0 °C | 7.76 g/cm³ Show Material materials with Density of 7.76 g/cm³ | |

350.0 °C | 7.74 g/cm³ Show Material materials with Density of 7.74 g/cm³ | |

400.0 °C | 7.72 g/cm³ Show Material materials with Density of 7.72 g/cm³ | |

450.0 °C | 7.7 g/cm³ Show Material materials with Density of 7.7 g/cm³ | |

500.0 °C | 7.68 g/cm³ Show Material materials with Density of 7.68 g/cm³ | |

550.0 °C | 7.66 g/cm³ Show Material materials with Density of 7.66 g/cm³ | |

600.0 °C | 7.64 g/cm³ Show Material materials with Density of 7.64 g/cm³ | |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | -100.0 °C | 217 GPa Show Material materials with Elastic modulus of 217 GPa |

20.0 °C | 212 - 212.48 GPa Show Material materials with Elastic modulus of 212 - 212.48 GPa | |

50.0 °C | 211.6 GPa Show Material materials with Elastic modulus of 211.6 GPa | |

100.0 °C | 207 - 209.25 GPa Show Material materials with Elastic modulus of 207 - 209.25 GPa | |

150.0 °C | 206.11 GPa Show Material materials with Elastic modulus of 206.11 GPa | |

200.0 °C | 199 - 202.48 GPa Show Material materials with Elastic modulus of 199 - 202.48 GPa | |

250.0 °C | 198.36 GPa Show Material materials with Elastic modulus of 198.36 GPa | |

300.0 °C | 192 - 194.14 GPa Show Material materials with Elastic modulus of 192 - 194.14 GPa | |

350.0 °C | 189.82 GPa Show Material materials with Elastic modulus of 189.82 GPa | |

400.0 °C | 184 - 185.51 GPa Show Material materials with Elastic modulus of 184 - 185.51 GPa | |

450.0 °C | 180.99 GPa Show Material materials with Elastic modulus of 180.99 GPa | |

500.0 °C | 175 - 176.48 GPa Show Material materials with Elastic modulus of 175 - 176.48 GPa | |

550.0 °C | 171.97 GPa Show Material materials with Elastic modulus of 171.97 GPa | |

600.0 °C | 164 - 166.97 GPa Show Material materials with Elastic modulus of 164 - 166.97 GPa | |

Unlock all property charts | ||

Elongation | 20.0 °C | 21 - 23 % Show Material materials with Elongation of 21 - 23 % |

Poisson's ratio | 20.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] |

50.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

100.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

150.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

200.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

250.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

300.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

350.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

400.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

450.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

500.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

550.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

600.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

Unlock all property charts | ||

Shear modulus | 20.0 °C | 82.6 GPa Show Material materials with Shear modulus of 82.6 GPa |

50.0 °C | 82.21 GPa Show Material materials with Shear modulus of 82.21 GPa | |

100.0 °C | 81.23 GPa Show Material materials with Shear modulus of 81.23 GPa | |

150.0 °C | 79.95 GPa Show Material materials with Shear modulus of 79.95 GPa | |

200.0 °C | 78.48 GPa Show Material materials with Shear modulus of 78.48 GPa | |

250.0 °C | 76.81 GPa Show Material materials with Shear modulus of 76.81 GPa | |

300.0 °C | 75.05 GPa Show Material materials with Shear modulus of 75.05 GPa | |

350.0 °C | 73.38 GPa Show Material materials with Shear modulus of 73.38 GPa | |

400.0 °C | 71.61 GPa Show Material materials with Shear modulus of 71.61 GPa | |

450.0 °C | 69.75 GPa Show Material materials with Shear modulus of 69.75 GPa | |

500.0 °C | 67.98 GPa Show Material materials with Shear modulus of 67.98 GPa | |

550.0 °C | 66.22 GPa Show Material materials with Shear modulus of 66.22 GPa | |

600.0 °C | 64.35 GPa Show Material materials with Shear modulus of 64.35 GPa | |

Unlock all property charts | ||

Tensile strength | 20.0 °C | 440 - 570 MPa Show Material materials with Tensile strength of 440 - 570 MPa |

Yield strength | 20.0 °C | 295 MPa Show Material materials with Yield strength of 295 MPa |

Yield strength Rp0.2 | 20.0 °C | 285 MPa Show Material materials with Yield strength Rp0.2 of 285 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.05E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.05E-5 1/K | |

20.0 °C | 1.15E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.15E-5 1/K | ||

100.0 °C | 1.21E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.21E-5 1/K | ||

200.0 °C | 1.27E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.27E-5 1/K | ||

300.0 °C | 1.32E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.32E-5 1/K | ||

400.0 °C | 1.36E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.36E-5 1/K | ||

500.0 °C | 1.4E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.4E-5 1/K | ||

600.0 °C | 1.44E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.44E-5 1/K | ||

Unlock all property charts | |||

Max service temperature, long | 0 - 530 °C Show Material materials with Max service temperature, long of 0 - 530 °C | ||

Melting point | 1382 - 1529 °C Show Material materials with Melting point of 1382 - 1529 °C | Typical for Molybdenum Steel | |

Specific heat capacity | -100.0 °C | 423 J/(kg·K) Show Material materials with Specific heat capacity of 423 J/(kg·K) | |

20.0 °C | 461 J/(kg·K) Show Material materials with Specific heat capacity of 461 J/(kg·K) | ||

100.0 °C | 479 J/(kg·K) Show Material materials with Specific heat capacity of 479 J/(kg·K) | ||

200.0 °C | 499 J/(kg·K) Show Material materials with Specific heat capacity of 499 J/(kg·K) | ||

300.0 °C | 517 J/(kg·K) Show Material materials with Specific heat capacity of 517 J/(kg·K) | ||

400.0 °C | 536 J/(kg·K) Show Material materials with Specific heat capacity of 536 J/(kg·K) | ||

500.0 °C | 558 J/(kg·K) Show Material materials with Specific heat capacity of 558 J/(kg·K) | ||

600.0 °C | 587 J/(kg·K) Show Material materials with Specific heat capacity of 587 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 52.1 W/(m·K) Show Material materials with Thermal conductivity of 52.1 W/(m·K) | |

100.0 °C | 51.2 W/(m·K) Show Material materials with Thermal conductivity of 51.2 W/(m·K) | ||

200.0 °C | 48.7 W/(m·K) Show Material materials with Thermal conductivity of 48.7 W/(m·K) | ||

300.0 °C | 45.5 W/(m·K) Show Material materials with Thermal conductivity of 45.5 W/(m·K) | ||

400.0 °C | 42.3 W/(m·K) Show Material materials with Thermal conductivity of 42.3 W/(m·K) | ||

500.0 °C | 39.1 W/(m·K) Show Material materials with Thermal conductivity of 39.1 W/(m·K) | ||

600.0 °C | 36 W/(m·K) Show Material materials with Thermal conductivity of 36 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 14.4 mm²/s Show Material materials with Thermal diffusivity of 14.4 mm²/s | |

100.0 °C | 13.2 mm²/s Show Material materials with Thermal diffusivity of 13.2 mm²/s | ||

200.0 °C | 11.7 mm²/s Show Material materials with Thermal diffusivity of 11.7 mm²/s | ||

300.0 °C | 10.3 mm²/s Show Material materials with Thermal diffusivity of 10.3 mm²/s | ||

400.0 °C | 9 mm²/s Show Material materials with Thermal diffusivity of 9 mm²/s | ||

500.0 °C | 7.5 mm²/s Show Material materials with Thermal diffusivity of 7.5 mm²/s | ||

600.0 °C | 6 mm²/s Show Material materials with Thermal diffusivity of 6 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 2E-7 - 2.16E-7 Ω·m Show Material materials with Electrical resistivity of 2E-7 - 2.16E-7 Ω·m |

50.0 °C | 2.37E-7 Ω·m Show Material materials with Electrical resistivity of 2.37E-7 Ω·m | |

100.0 °C | 2.5E-7 - 2.68E-7 Ω·m Show Material materials with Electrical resistivity of 2.5E-7 - 2.68E-7 Ω·m | |

150.0 °C | 3.02E-7 Ω·m Show Material materials with Electrical resistivity of 3.02E-7 Ω·m | |

200.0 °C | 3.24E-7 - 3.39E-7 Ω·m Show Material materials with Electrical resistivity of 3.24E-7 - 3.39E-7 Ω·m | |

250.0 °C | 3.8E-7 Ω·m Show Material materials with Electrical resistivity of 3.8E-7 Ω·m | |

300.0 °C | 4.12E-7 - 4.25E-7 Ω·m Show Material materials with Electrical resistivity of 4.12E-7 - 4.25E-7 Ω·m | |

350.0 °C | 4.74E-7 Ω·m Show Material materials with Electrical resistivity of 4.74E-7 Ω·m | |

400.0 °C | 5.14E-7 - 5.27E-7 Ω·m Show Material materials with Electrical resistivity of 5.14E-7 - 5.27E-7 Ω·m | |

450.0 °C | 5.83E-7 Ω·m Show Material materials with Electrical resistivity of 5.83E-7 Ω·m | |

500.0 °C | 6.33E-7 - 6.42E-7 Ω·m Show Material materials with Electrical resistivity of 6.33E-7 - 6.42E-7 Ω·m | |

550.0 °C | 7.08E-7 Ω·m Show Material materials with Electrical resistivity of 7.08E-7 Ω·m | |

600.0 °C | 7.69E-7 - 7.78E-7 Ω·m Show Material materials with Electrical resistivity of 7.69E-7 - 7.78E-7 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.12 - 0.2 % Show Material materials with Carbon of 0.12 - 0.2 % |

Chromium | 0.3 % Show Material materials with Chromium of 0.3 % |

Copper | 0.3 % Show Material materials with Copper of 0.3 % |

Manganese | 0.4 - 0.9 % Show Material materials with Manganese of 0.4 - 0.9 % |

Molybdenum | 0.25 - 0.35 % Show Material materials with Molybdenum of 0.25 - 0.35 % |

Nickel | 0.3 % Show Material materials with Nickel of 0.3 % |

Phosphorus | 0.03 % Show Material materials with Phosphorus of 0.03 % |

Silicon | 0.35 % Show Material materials with Silicon of 0.35 % |

Sulfur | 0.01 - 0.015 % Show Material materials with Sulfur of 0.01 - 0.015 % |